IJCER (www.ijceronline.com) International Journal of computational Engineering research
1.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 5Study of Transient Temperature Distribution in a Friction Welding Process and its effects on its Joints. Sirajuddin Elyas Khany1, K.N.Krishnan2, Mohd Abdul Wahed3 1 Associate Professor, 2Professor, 3 Graduate Student, MED, MJCET, Hyderabad, India.Abstract:In Materials like Stainless Steel 304 and Eutectoid Steel, microstructure is affected during the process of friction welding leadingto variation in Hardness and strength. In the present Study, the transient temperature distribution in a friction welded Joint ofsimilar materials in one dimension (uniaxial direction) is studied. A numerical method based on thermal networking is used toestimate the transient temperature distribution. Microstructure variation of specimen is also studied. The preliminary predictionsare compared to actual experimental data from welding conducted under identical conditions. The results are shown to be in fairagreement. The numerical method proposed in this work provides guidance in weld parameter development and allows betterunderstanding of the friction welding process.Key Words: Friction Welding, Numerical Method, Temperature Distribution, Microstructure and Hardness.Introduction: In the present study, the friction welding technology used is one in which the rotational motion of the work pieces isstopped after the pressure has been applied for a very short period of time. During the process, the frictional heat is generated inthe interface till plastic deformation stage is reached. Then, the rotation is stopped to let the welded joint cool down under freeconvection. Peak joint temperature and the temperature profile in the region near the joint have a significant impact on the flashformation, the extend of heat effected zones and the joint strength. The thermal effects of the friction welding are observed tohave lowered the hardness of the welded materials compared to the parent materials. Heating and cooling rates are closelyrelated to the joint temperature and directly influence the residual stresses developed in the joint. Therefore, it is vital to have ameans of rapidly and accurately estimating the peak joint temperature and cooling rates based on input parameters. A numericalmethod is developed, simulating the friction welding to quickly visualize the process specific responses to define the quality ofthe weld. An analysis of these phenomena is helpful in improving both the method and strength of the bonds in the weldingprocess. Mechanical evaluation and thermal modeling of friction welding of mild steel and aluminium is described by HazmanSeli et al (1).A new friction law of modeling of continuous drive friction welding and application to1045 steel welds is presentedby Balsubramaniam et al (2). Thermically evaluation and modeling of friction welding is presented by Ahmet Can et al (3).Estimation of heat generation at the interface of cylindrical bars during friction process is presented by Wen-lih Chen et al (4).Experimental and numerical analysis of the friction welding process for the 4340 steel and mild steel combinations is describedby Akbari Mousavi et al (5). Numerical simulation of linear friction welding of titanium alloy: Effects of processing parametersis presented by Wen-ya li et al (6). Thermo-mechanical and diffusion modeling in the process of ceramic-metal friction weldingis done by Jolanta Zimmerman et al (7). Dynamic simulation of the temperature field of stainless steel laser welding is describedby Han GuoMing et al (8). Temperature and stress distribution in ultrasonic metal welding—An FEA-based study is presentedby S. Elangovan et al (9). The focus of the present paper is to understand the thermal effects on the weld work piece and analyze the transienttemperature profiles in the welded rods during friction welding. The numerical method is applied in obtaining the solution andthe resulting temperature fields are compared with experimental data.Issn 2250-3005(online) September| 2012 Page 1645
2.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 5Materials and Method:A continuous drive friction welding as shown in fig. 1 was used to produce a weld between stainless steel- stainless steel andeutectoid steel- eutectoid steel rods of diameter 15mm and length 80mm.Fig. 1 Scheme of continuous drive friction welding Fig. 2. Axial pressure and rotational velocity used in the experiment.The changes of load and rotational speed in time during the process are shown in Fig. 2. The characteristic phases are marked. Inphase (A), axial load and rotational speed of the steel rod were applied and the two rods were brought near the joined surfaces.Then in phase (B), the two rods underwent friction heating at the interface. When the rotational speed was stopped in phase (C),the frictional heated surface cooled down and at the same time, the upsetting under increased pressure occurred. Finally in phase(D), the pressure remained constant until the axial pressure is released. The chemical composition of the Stainless steel and Eutectoid Steel employed in this study are summarized in Table 1. Thetemperature changes during the friction welding process are measured at a time by two k-type thermocouples attached to thestationary rod at a distance of 7mm, 14mm, 21mm and 28mm from the interface. The axial pressure is applied from the fixed endgradually. The temperature profiles are recorded at specific time intervals, till the welding is complete. The locations of thethermocouple is shown in fig.3. Fig. 3. The locations of the thermocouple placement 7, 14, 21 and 24mm from the interface, respectively.For metallurgical examination the welded sample is sectioned perpendicular to the weld interface. The joint sample is groundand polished. Microstructure is obtained using optical microscope. The Rockwell hardness is measured at the point of highesttemperature from the interface (i.e. at 7mm from the interface). Table 1 (Chemical composition of stainless steel 304 and eutectoid steel by wt %) Element C Mn P Cu Mo S Cr N Si Fe Ni S.S(304) 0.08 20 0.045 0.75 0.75 0.05 20 0.10 1.00 Bal 10.5 Eutectoid steel 0.80 0.7 0.04 ------ ------ 0.05 ----- ------ ------ ----- ---------Issn 2250-3005(online) September| 2012 Page 1646
3.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 53. Mathematical Modeling:3.1. General assumptions for the analysis of friction welding: Heat generation and pressure across the interface are assumed to be uniform. There is no heat exchange between the end faces of the steel rods and the environment. The steel rods are assumed to be homogenous and isotropic. The heat input is considered constant throughout the process.3.2. Thermal analysis:During friction welding, the temperature in the weld region rises sharply due to extreme frictional heat and plastic deformationof the steel rod within a very short time. To calculate the temperature profile, the heat transfer analysis is undertaken byconsidering the frictional heat generation at the interface and heat loss to the surroundings by conduction and convection.3.2.1. Frictional heat generation model:Based on the assumption that force distribution remains constant, the frictional heat is deduced through the following analyticalmethod.First, a micro annulus with an inner radius r and a width dr in the friction surface is defined as in Fig. 4.The constant pressure acting on the entire surface is given by p. The area of the micro annulus is dA = (2¶r) dr. Transforming thepressure equation into a differential characterization of the area dA, the following equation is obtained for the differential force,dF, acting on the area dA.dF = p dA = 2p¶r dA (1) Fig. 4. Friction interface sketch.Since dF is equivalent to the equal and opposite normal force acting on dA, the differential frictional force, dF f, can be specifiedas dFf = µdF = 2µp¶r dr (2)Where µ is friction coefficient. It is known that the tangential velocity, vT at any point on the element is the same, vT = r (3)Where ω is angular velocity.The differential power that is exerted to rotate the annulus area dA is dP = dFf (vT) = 2µp¶r2ω dr (4)Therefore, by integrating Eq. (4) with respect to r, the definition for the frictional heating power generation is obtained as P =0⌡R 2µp¶r2ω dr = (2/3) µp¶R3ω (5)The heat flux (q) generated by friction at the annulus is given asIssn 2250-3005(online) September| 2012 Page 1647
4.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 5 q(r) = dP/dA = 1.6µpωr (6)3.3. Heat transfer:The fundamental non-steady equation of Fourier’s heat conduction in the coupled thermo-mechanical problem can be expressedas follows: ∂T/∂t + u (∂T/∂x) = 1/ρCp ∂/∂x (k∂T/∂x) − hP/ρCpA (T − To) + q˙ (7)where T is temperature, To is the ambient temperature around the rod, u is the shortening velocity, ρ is the material density, Cp isthe specific heat capacity, A is the cross-sectional area, P is the perimeter of the rod, k is the thermal conductivity, h is theconvection coefficient, x is the distance from the weld interface and t is time.For simplicity, Eq. (7) can be rewritten as ∂T/∂t + u (∂T/∂x) = α (∂2T/∂x2) − β (T − To) + q˙ (8)Where α = k/ρCp and β = hP/ρCpA.In this one-dimensional equation, the convection term on the right-hand side of the equation accounts for heat conduction andheat lost through convection along the lateral surfaces of the two components. It is assumed that there is no heat lost throughradiation at the frictional interface. The problem of heat conduction in the whole process of friction welding determined bymeans of Eq. (8) was, thus, simplified to the calculation of temperature field, T = T(x,t). The calculation of the temperature ofthe friction welding process is carried out in two stages. The first stage is the heating part while the second is the coolingprocess. The initial and boundary conditions when solving Eq. (8) are expressed based on the two stages.3.3.1. Heating stage:The temperature distribution is calculated for heating separately for the rod of length(L) by assuming common average heatgenerated at the interface. For the heating stage, the initial and boundary conditions for the simplified equation (8) are derived asT(x, th) = To, for th = 0 (9)−k (∂T/∂x) = q, x = 0 for th > 0 and (10)−k (∂T/∂x) = h (T − To), x = L, for th > 0 (11) Where th is the heating or frictional time, To is the initial temperature of the specimen, q is the surface heat flux generated at thefriction surface (x = 0).3.3.2. Cooling stage (welded):At this stage the rods have been joined and considered as one new rod for the calculation, where the initial and boundaryconditions for the simplified equation (8) are derived asT (xj, tc) = Tn, for tc = 0 and (12)Ks (∂T/∂x) = ha (Ts − To), xj = 0, for tc > 0 (13)Where xj is the distance from left end of the joined rods, t c is the cooling time, k is the thermal conductivity of the steel, and T isthe temperatures of the free surfaces of the steel. Tn is the last temperature profile from the previous heating stage. The onlyunknown in the equation presented above is the shortening velocity (u) which is assumed to be zero. The calculation of thetemperature is carried out using FORTRAN. The properties of Stainless steel 304 and Eutectoid steel are listed in Table 2. As shown below. Properties Stainless steel 304 Eutectoid steel Density(kg/m3) 7900 7840 Thermal conductivity(w/mk) 15 46 Specific heat(j/kg k) 477 470 o Melting Point 1371 - 1532 CIssn 2250-3005(online) September| 2012 Page 1648
5.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 54. Results and discussion: The experimental study is done on a continuous drive friction welding machine. The friction welding parameterswere 490 and 790rpm rotational speed, 5-8 bar friction pressure and 11-15 bar upsetting pressure. Hardness profiles of parentand welded samples are determined. A one-dimensional numerical model for temperature profiles of this process is proposed andsolved using FORTRAN program developed in the data processing center of Muffakham – Jah – College of Engg. & Tech.Hyderabad4.1 Microstructure Variation: Fig.5 Microstructure variation of S.S 304 before and after friction welding at 675x.The microstructure consists of single phase austenite. The microstructure is completely austenite of equiaxed uniform grainswithin the grains, slip bands are seen and the grain boundaries are clear. Precipitate of alloy carbides is noticed. Due to chemicalcomposition deposition alloy carbides are seen which are not refined before friction welding. Subjected to friction welding at 613oC (i.e. at a distance of 7mm, the highest peak temperature from the interface) it isobserved that there is grain refinement along with the precipitation of carbides. Before friction welding After friction welding Grain size ASTM: 6 Grain size ASTM: 7 Fig.6 Microstructure variation of Eutectoid steel before and after friction welding at 675x.Microstructure reveals 100% pearlite in the form of lamella structure (alternate bands of cementite and ferrite) before frictionwelding. Dark areas are pearlite and light areas are ferrite. Microstructure reveals 100% pearlite which is more refined after friction welding and can be seen in the form of lamellastructure (alternate bands of cementite and ferrite). In this study the highest temperature reached is 600oC (i.e. at a distance of 7mm from the weld interface) in both thesteel rods. More changes in the microstructure are not expected because the temperature is within the range of eutectoidtemperature (i.e. below 723oC).Issn 2250-3005(online) September| 2012 Page 1649
6.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 54.2 Hardness Profile: Fig. 7a and 7b shows the result of the Rockwell hardness test for S.S 304 and Eutectoid steel. The hardness value ischecked for both the steel rods at distance of 7, 14, 21 and 28mm of welded part and is found to be lower at the first node (i.e. at7mm) than that of its parent part. This reduction could be due to the thermal effect in the welded steel. Due to normalizing thehardness is increasing as the distance from the weld is increasing. In stainless steel 304, hardness is increasing gradually and ineutectoid steel rapidly this, difference in both the steel rods is due to the refinement of grain structure and homogenization of themicrostructure due to normalizing. Fig.7a Results of the Rockwell hardness test for Stainless steel 304 Fig.7b Results of the Rockwell hardness test for Eutectoid steel.Due to normalizing, hardness is increasing in both the steel rods, and as the hardness is increases, strength also increases.4.3 Heating and cooling stage: The transient heating and cooling temperature distribution for steel rods are shown in Fig. (9a – 9p).From thetemperature distribution, it is seen that the calculated peak temperature in heating for stainless steel at 90sec and 40sec is about613oC and 378oC and for eutectoid steel is 578oC and 270oC at 200sec and 70sec, peak temperatures in heating for steel rods areobtained at a distance of 7mm from the interface at 490 and 790rpm with constant heat generated. Cooling starts of as the entireprocess, where the last heating temperature profile has been utilized. Similarly transient heating and cooling temperatures areobtained for similar parameters at 14, 21 and 28mm from the interface. The temperature increases rapidly at the interface, andgradually towards the end of the steel rods. The transient heating and cooling temperature distribution in eutectoid steel is faster.This is due to the higher thermal conductivity in eutectoid steel compared to that in stainless steel. Due to the lower thermalconductivity stainless steel is taking less time for welding when compared to eutectoid steel. As the speed (rpm) is increasingtemperature as well as time is decreasing in both the steel rods, but the variation is nearly similar. The difference can beattributed to accomodating the heat losses at the interface in the analytical model. The thermal heating profile likely exhibits the interaction between the frictional heating power and the frictionalcharacteristics on the surface. However, in a real situation, the pressure distribution is not uniform with time as the two workpieces move in sinusoidal fashion. While the axial force remains constant, the area of contact between the two work pieceschanges with movement and leads to the oscillation of the axial pressure at the interface. Therefore, altering the axial pressureduring every cycle owing to the variation of contact area causes the frictional heat input to fluctuate as well. The frictioncoefficient varies widely with temperature. The increase in the temperature softens the ductile material and brings about deepploughing on the contact surfaces. Then, the contact seems to have been altered into a polishing-like action and the frictioncoefficient is dramatically reduced. The inaccuracy in the calculation was attributed to the assumption of constant coefficient offriction and pressure for the analytical constant heat generation.Issn 2250-3005(online) September| 2012 Page 1650
7.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 5Fig.9a Time–temperature profiles at a distance of 7mm from the weld interface for numerical and experimental data of stainless steel at 490rpm. Fig.9b Time–temperature profiles at a distance of 14mm from the weld interface for numerical and experimental data of stainless steel at 490rpmFig.9c Time–temperature profiles at a distance of 21mm from the weld interface for numerical and experimental data of stainless steel at 490rpm Fig.9d Time–temperature profiles at a distance of 28mm from the weld interface for numerical and experimental data of stainless steel at 490rpmIssn 2250-3005(online) September| 2012 Page 1651
8.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 5Fig.9e Time–temperature profiles at a distance of 7mm from the weld interface for numerical and experimental data of stainless steel at 790rpmFig.9f Time–temperature profiles at a distance of 14mm from the weld interface for numerical and experimental data of stainless steel at 790rpmFig.9g Time–temperature profiles at a distance of 21mm from the weld interface for numerical and experimental data of stainless steel at 790rpm Fig.9h Time–temperature profiles at a distance of 28mm from the weld interface for numerical and experimental data of stainless steel at 790rpmIssn 2250-3005(online) September| 2012 Page 1652
9.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 5Fig.9i Time–temperature profiles at a distance of 7mm from the weld interface for numerical and experimental data of eutectoid steel at 490rpmFig.9j Time–temperature profiles at a distance of 14mm from the weld interface for numerical and experimental data ofeutectoid steel at 490rpm Fig.9k Time–temperature profiles at a distance of 21mm from the weld interface for numerical and experimental data of eutectoid steel at 490rpm Fig.9l Time–temperature profiles at a distance of 28mm from the weld interface for numerical and experimental data of eutectoid steel at 490rpmIssn 2250-3005(online) September| 2012 Page 1653
10.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 5 Fig.9m Time–temperature profiles at a distance of 7mm from the weld interface for numerical and experimental data of eutectoid steel at 790rpm Fig.9n Time–temperature profiles at a distance of 14mm from the weld interface for numerical and experimental data of eutectoid steel at 790rpm Fig.9o Time–temperature profiles at a distance of 21mm from the weld interface for numerical and experimental data of eutectoid steel at 790rpm Fig.9p Time–temperature profiles at a distance of 28mm from the weld interface for numerical and experimental data of eutectoid steel at 790rpmIssn 2250-3005(online) September| 2012 Page 1654
11.
International Journal Of Computational Engineering Research (ijceronline.com) Vol. 2 Issue. 54.4. Verification of the predicted profile with experimental data:The verification of the predicted temperature distribution of the welded rods are presented in Fig.9. for locations 7, 14, 21 and28mm from the interface. The computed temperature profile does not exactly match with the experimental data. However, thetrend of the profiles shown is similar. The predicted heating and cooling temperature profiles of the friction welding are in fair agreement with theexperimental temperature profiles. The heating and cooling rates of the process are approximately calculated around 138 ◦C/sand 45 ◦C/s, respectively. After the rotation of the steel rod is stopped, the temperature profile increases and decreases withlower gradients compared to the measured temperature profile. The discrepancy of the two temperature profiles is mostlyattributed to the static nature of the model. After 10 s, the difference is quite significant, most probably because the proposedmodel does not consider the entire work pieces for calculation. In the friction welding process, at every moment of the frictionphase, the plasticized material is expelled out of the faying surface due to the mutual movement of the mating surfaces. Incontrast, the numerical model is simply based on the static analysis in which the heat generated at the interface is assumed to betotally transferred to the base materials with no flash formed (zero axial shortening assumption). Therefore, the relativemovement (rubbing) of the two parts, which is the main reason for ejecting softened material from the rubbing surface, is notconsidered in the model. Apart from that, the errors could also come from the temperature measurement since operation ismanual. Even though inaccurate, these details are still useful in friction welding process study, especially in explaining the heataffected zone which eventually affects the strength of the joint. Hence, the proposed model provides some parameterdevelopment and allows better understanding of the friction welding process.5. Conclusions: Bonds of stainless steel vs stainless steel and eutectoid steel vs eutectoid steel are achieved in the friction weldingprocess. The welded materials have lower hardness measured at a distance of 7mm from the interface compared to their parentmaterials due to thermal effects of the friction welding. But as the distance from the interface is increasing hardness is increasingdue to normalizing and this has been also compared with CCT diagram. A one-dimensional numerical model for continuousdrive friction welding was developed according to the characteristics of the friction welding process. It is introduced to enable abetter understanding of the process. The predicted transient heating and cooling temperature profile of the friction welding is infair agreement with the experimental temperature distribution.Acknowledgements: The authors gratefully acknowledge the co-operation and help extended by Mr. Mansur from metal cutting laboratory andMr. Hashmi from metallurgy laboratory in carrying out the experiment during this research work.References: [1.] Hazman Seli, Ahmad Izani Md.Ismail, Endri Rachman, Zainal Arifin Ahmad.(2010) Mechanical evaluation & thermal modeling of friction welding of mild steel & aluminium. Journal of materials processing technology 210 (1209-1216). [2.] Vikram Balasubramaniana; Youlin Lib; Tim Stotlerc; Jeff Cromptonc; Alfred Soboyejoa; Noriko Katsubea;Wolé Soboyejo.(1999). A New Friction Law for the Modelling of Continuous Drive Friction Welding: Applications to 1045 Steel Welds, materials & manufacturing process, 14:6, (845-860). [3.] ahmet CAN, Mumin SAHIN & Mahmut KUCUK(2009).Thermically Evaluation & modeling of friction welding,strojarstvo 51(1) (5-13). [4.] Wen-lih chen, Yu-ching yang, Shao-shu chu(2009).Estimation of heat generation at the interface of cylindrical bars during friction process), Applied thermal Engineering 29 (351-357). [5.] s.a.a.akbari mousavi & a. rahbar kelishami(2008), Experimental & numerical analysis of the friction welding process for the 4340 steel & mild steel combinations. Welding research 178-186s(vol.87). [6.] Wen-ya li, Tiejun Ma, Jinglong Li(2010), Numerical simulation of linear friction welding of titanium alloy: Effects of processing parameters, Materials & Design 31(1497-1507). [7.] Jolanta Zimmerman, wladyslaw wlosinski, zdzislaw R Lindemann Thermo-mechanical & diffusion modeling in the process of ceramic-metal friction welding(2009), Journal of materials processing Technology 209, (1644-1653). [8.] Han GuoMing *, Zhao Jian, Li JianQang(2007), Dynamic simulation of the temperature field of stainless steel laser welding, Material & Design 28 (240-245). [9.] S. Elangovan, S. Semeer, K. PrakasanTemperature and stress distribution in ultrasonic metal welding—An FEA-based study (2009),Journal of material processing Technology 209,(1143–1150).Issn 2250-3005(online) September| 2012 Page 1655
Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.
Be the first to comment